| ||Format||Pages||Price|| |
|8||$50.00||  ADD TO CART|
|Hardcopy (shipping and handling)||8||$50.00||  ADD TO CART|
|Standard + Redline PDF Bundle||16||$60.00||  ADD TO CART|
Significance and Use
5.1 Continuous fiber-reinforced ceramic composites are candidate materials for structural applications requiring high degrees of wear, erosion, corrosion resistance, and damage tolerance at high temperatures.
5.2 The 1D and 2D CFCCs are highly anisotropic and their transthickness tensile and interlaminar shear strength are lower than their in-plane tensile and in-plane shear strength, respectively.
5.3 Shear tests provide information on the strength and deformation of materials under shear stresses.
5.4 This test method may be used for material development, material comparison, quality assurance, characterization, and design data generation.
5.5 For quality control purposes, results derived from standardized shear test specimens may be considered indicative of the response of the material from which they were taken for given primary processing conditions and post-processing heat treatments.
1.1 This test method addresses the uniaxial compression of a double-notched test specimen to determine interlaminar shear strength of continuous fiber-reinforced ceramic composites (CFCCs) at elevated temperatures. Failure of the test specimen occurs by interlaminar shear between two centrally located notches machined halfway through the thickness of the test specimen and spaced a fixed distance apart on opposing faces (see ). Test specimen preparation methods and requirements, testing modes (force or displacement control), testing rates (force rate or displacement rate), data collection, and reporting procedures are addressed.
FIG. 1 Schematic of Uniaxial Compression of Double-Notched Test Specimen for the Determination of Interlaminar Shear Strength of CFCCs
1.2 This test method is used for testing advanced ceramic or glass matrix composites with continuous fiber reinforcement having a laminated structure such as in unidirectional (1D) or bidirectional (2D) fiber architecture (lay-ups of unidirectional plies or stacked fabric). This test method does not address composites with nonlaminated structures, such as (3D) fiber architecture or discontinuous fiber-reinforced, whisker-reinforced, or particulate-reinforced ceramics.
1.3 Values expressed in this test method are in accordance with the International System of Units (SI) and .
1.4 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use. Specific precautionary statements are noted in and .
1.5 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
C1145 Terminology of Advanced Ceramics
C1292 Test Method for Shear Strength of Continuous Fiber-Reinforced Advanced Ceramics at Ambient Temperatures
D695 Test Method for Compressive Properties of Rigid Plastics
D3846 Test Method for In-Plane Shear Strength of Reinforced Plastics
D3878 Terminology for Composite Materials
D6856/D6856M Guide for Testing Fabric-Reinforced Textile Composite Materials
E4 Practices for Force Verification of Testing Machines
E6 Terminology Relating to Methods of Mechanical Testing
E122 Practice for Calculating Sample Size to Estimate, With Specified Precision, the Average for a Characteristic of a Lot or Process
E220 Test Method for Calibration of Thermocouples By Comparison Techniques
E230/E230M Specification for Temperature-Electromotive Force (emf) Tables for Standardized Thermocouples
E337 Test Method for Measuring Humidity with a Psychrometer (the Measurement of Wet- and Dry-Bulb Temperatures)
ICS Number Code 81.060.30 (Advanced ceramics)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM C1425-19, Standard Test Method for Interlaminar Shear Strength of 1D and 2D Continuous Fiber-Reinforced Advanced Ceramics at Elevated Temperatures, ASTM International, West Conshohocken, PA, 2019, www.astm.orgBack to Top